Review Removal of Heavy Metals and Metalloids from Water Using Drinking Water Treatment Residuals as Adsorbents: A Review
Magdalena Wołowiec 1,*, Małgorzata Komorowska-Kaufman 2 , Alina Pruss 2 , Grzegorz Rzepa 1 and Tomasz Bajda 1,*
1 Faculty of Geology, Geophysics and Environmental Protection, AGH University of Science and Technology, al. A. Mickiewicza 30, 30-059 Krakow, Poland 2 Institute of Environmental Engineering, Poznan University of Technology, Faculty of Civil and Environmental Engineering, ul. Berdychowo 4, 60-965 Pozna´n,Poland * Correspondence: [email protected] (M.W.); [email protected] (T.B.); Tel.: +48-500-032-026 (M.W.); +48-12-617-52-32 (T.B.) Received: 18 June 2019; Accepted: 13 August 2019; Published: 14 August 2019
Abstract: Heavy metal contamination is one of the most important environmental issues. Therefore, appropriate steps need to be taken to reduce heavy metals and metalloids in water to acceptable levels. Several treatment methods have been developed recently to adsorb these pollutants. This paper reviews the ability of residuals generated as a by-product from the water treatment plants to adsorb heavy metals and metalloids from water. Water treatment residuals have great sorption capacities due to their large speciﬁc surface area and chemical composition. Sorption capacity is also aﬀected by sorption conditions. A survey of the literature shows that water treatment residuals may be a suitable material for developing an eﬃcient adsorbent for the removal of heavy metals and metalloids from water.
Keywords: adsorption; arsenic; pollutants; water treatment sludges
1. Introduction Heavy metals are a group of trace elements that include metals and metalloids, such as arsenic, cadmium, chromium, cobalt, copper, iron, lead, manganese, mercury, nickel, tin, and zinc. They have a relatively high density of over 4 106 mg/L. The metal ions are known to contaminate the soil, × atmosphere, and water systems and are poisonous even in very low concentrations . There are two main sources of heavy metals in water—natural and anthropogenic. Natural sources comprise volcanic activities, soil erosion, activities of living organisms, and weathering of rocks and minerals, whereas anthropogenic sources include landﬁlls, fuel combustion, street run-oﬀs, sewage, agricultural activities, mining, and industrial pollutants, such as textile dyes . Heavy metals are classiﬁed as toxic and carcinogenic, they are capable of accumulating in tissues and cause diseases and disorders (Table1).
Minerals 2019, 9, 487; doi:10.3390/min9080487 www.mdpi.com/journal/minerals Minerals 2019, 9, 487 2 of 17
Table 1. Comparison of selected heavy metals, their anthropogenic sources, provisional maximum tolerable daily intake (PMTDI) according to WHO, and symptoms and diseases.
Heavy Metal Anthropogenic Sources PMTDI (mg/L) Symptoms and Diseases References Pesticides, biosolids, disposal of industrial wastes, mining activities, feed additives, insecticides, ceramics, veterinary Arsenicosis, cancers of the bladder, skin, lungs, As 0.01 [3,4] medicine, metallurgy, herbicides, electronic components, and kidneys electrical generation, tanning, and textile Petroleum reﬁning, electroplating and alloying industry, Emphysema, hypertension, nephropathy, diabetes Cd nickel–cadmium batteries, coal combustion, 0.003  mellitus, skeletal malformation plastic stabilizers Pigments, chemicals, electroplating, coasting operations, Allergic reactions, skin rash, nose irritations, nosebleed, Cr wood treatment, data storage, textiles and leather 0.05 ulcer, weakened the immune system, genetic material [6,7] tanning, metallurgy alteration, kidney and liver damage, cancer Preparation of semiconductors, nuclear medicine, enamel and painting on glass, grinding wheels, porcelain, Paralysis, diarrhea, lung irritation, bone defects, low Co 0.002  hydrometers, electroplating, aerospace materials, blood pressure, genetic changes in cells Li-ion batteries Mining operations, chemical, and pharmaceutical Menkes, Wilson, Alzheimer’s, Parkinson’s diseases, Cu 1.5  equipment, kitchenware, paper manufacturing damages for eye and liver, vomiting, cramps, convulsions Hemochromatosis, eyes disorder, cancer, and Fe Iron and steel industries, mining, metal corrosion No guideline  heart diseases Fuels, manufacturing of electronic products, metal Reproductive system damage, central nervous system Pb processing, painting pigments, electroplating, leather 0.01  damage, liver and kidneys diseases tanning and mining Mining operations, tanneries, dental ﬁlling, solders, Hg Kidneys, lungs and eyes diseases, skin dermatitis, nervous Hg vapor lamps, metal plating facilities, amalgamation, 0.001  system dysfunction catalysts, pharmaceuticals, rectiﬁers, fungicides Corrosion of iron pipes, production of manganese steels, Lethargy, tremors, psychological disturbances, Mn 0.5  ferromanganese alloys respiratory infections Nickel steel, non-ferrous alloys, superalloys, Anemia, diarrhea, encephalopathy, hepatitis, lung and electroplating, alnico magnets, coinage, microphone kidney damage, gastrointestinal distress, pulmonary Ni 0.02 [14,15] capsules, rechargeable batteries, plating on plumbing ﬁbrosis, renal edema, skin dermatitis, central nervous ﬁxtures, catalysts, dental and surgical prostheses system dysfunction. Batteries, pigments, Zn alloys, rubber industry, chemical Depression, lethargy, respiratory incapacitation, appetite Zn 3  industry, paints, cans, anti-corrosion coating loss, diarrhea, headaches Minerals 2019, 9, 487 3 of 17
Contamination of aquatic systems is a serious environmental issue and therefore the development of an eﬃcient and suitable technology to remove heavy metals from aqueous solutions is necessary. Several methods have been used to remove heavy metals from contaminated water. They include chemical precipitation [17,18], ion exchange [19,20], adsorption [21,22], membrane ﬁltration [23,24], reverse osmosis [25,26], solvent extraction , and electrochemical treatment [28,29]. Many of these methods suﬀer from high capital and operational costs. Adsorption seems to be one of the best-suited methods, due to its high eﬃciency, low-cost, and ease of operation. Various adsorbents, such as carbon foam , activated carbon , zeolite , clay minerals [33,34], organic polymers , and biochar , and many waste materials, such as ﬂy ash , reused sanding wastes , biomass , and water treatment residuals (WTRs) [40,41], have been used for the removal of heavy metals by adsorption. The most eﬀective heavy metal adsorbents, especially for arsenic, are adsorbents based on metal oxides (Fe, Al, Mn oxides), such as WTRs, bog iron ores , ferrihydrite , goethite , layered double hydroxide (LDH) , Sn/Ti-Mn binary metal oxides [46,47], Al/Fe oxide-oxyhydroxide composite powders , and red mud . Using waste products as adsorbents provides many beneﬁts. It decreases the cost of removing metals from water, as well as being conducive to decreasing amounts of residuals which are accumulated in the environment. WTRs, sometimes referred to as water treatment sludge or waterworks sludge, are by-products generated by drinking water treatment plants. Each year, several million tons of WTRs are produced [50–54]. Their disposal is problematic and expensive due to environmental restrictions and has provided the impetus for research into their reuse . Proper handling of huge amounts of WTRs in an economical and environmentally friendly manner is, therefore, a very signiﬁcant issue. The feasibility of managing WTRs is determined by their chemical composition and properties, which are diversiﬁed due to the wide variation in the type and chemical composition of raw water, geology, and hydrogeology of the intake area, as well as water treatment technology. In recent years, an increasing number of studies have addressed the use of WTRs to remove pollutants from aqueous solutions. Most of the research is focused on the precipitation of phosphorous from wastewater [56,57]. Researchers indicate that WTRs are characterized by good sorption properties [51,58–61]. The aim of the present research was to present a review of the studies that have evaluated WTRs as heavy metals sorbents.
2. Materials and Methods
2.1. Materials In this review, the authors provide collected researches concerning the sorption capacity for heavy metals and metalloids of post-coagulation residuals of surface water treatments (SWTRs) and residuals of deironing and demanganization processes of groundwater treatments (GWTRs) as there is no similar review. The comparison of research is crucial due to the necessity to ﬁnd the most eﬀective methods of using sludges as sorbents. The authors reviewed publications describing the characteristics and sorption properties of SWTRs or GWTRs. They focused on the research papers reported within 10 years as there is also an increase in interest in the use of sludge from water treatment. The methodology and parameters of sorption and results as a function of time, pH, sorbent dose, initial concentration, and temperature were presented. Additionally, the parameters at which the sorption was most eﬀective were indicated. The authors compared the sorption values of individual heavy metals and metalloids on SWTRs and GWTRs. They also described the part of their research on the sorption capacity of heavy metals and metalloids on GWTRs.
2.2. Authors’ Research GWTRs generated as a by-product of the deironing process of underground water were used in the experiments. The sample was collected from a water treatment station in Wielkopolska Minerals 2019, 9, 487 4 of 17
Voivodship, Poland. Samples of GWTRs were dried and ground in a mortar and sieved using a 1 mm sieve to remove large particles. The phase composition was determined by X-ray powder diﬀraction (RIGAKU SmartLab Diﬀractometer, RIGAKU, Tokyo, Japan). To observe the surface and performing microanalyses the electron microscopy using a variable pressure ﬁeld emission scanning electron microscope (FEI Quanta 200, Graz, Austria) was used. The SBET was determined from N2 gas adsorption/desorption isotherms at 77 K after outgassing for 12 h at 373 K using an ASAP 2020 apparatus (Micrometrics, Norcross, GA, USA). Static sorption experiments were carried at a Liquid to Solid (L/S) ratio equal to 1:20 (5 mL solution + 100 mg sample). The reaction time was 24 h. The pH of the stock solution was not regulated. The experiments were conducted at room temperature. The inﬂuence of Cd(II), Pb(II), Zn(II), Cu(II), Cr(III), Cr(VI) and As(V) concentration (0.1, 1, 10, and 100 mM/L) on the sorption capacity was investigated. The source of ions was analytical grade reagents: Cd(NO ) 4H O; 3 2· 2 Pb(NO ) ; Zn(NO ) 6H O; CuN O 3H O; K Cr O ; CrN O 9H O; Na HAsO 7H O, respectively. 3 2 3 2· 2 2 6· 2 2 2 7 3 9· 2 2 4· 2 The concentrations of selected heavy metals and metalloids in an equilibrium solution was analyzed by atomic absorption spectroscopy (AAS) (SavantAA GBC Scientiﬁc Equipment, Braeside, Australia) and UV-Vis spectrophotometry (Hitachi U-1800, Berkshire, UK).
3. Material Characterization In this review, some SWTRs and GWTRs were compared. The chemical composition and properties of the WTRs are diversiﬁed and depend on their origin (surface or groundwater) and chemical composition of the treated water and/or methods and materials used for water treatment.
3.1. Post-Coagulation Residuals Usually, surface water carries suspended and colloidal solids, organic compounds, and other contaminants. Water treatment includes processes, such as coagulation, ﬂocculation, sedimentation, and ﬁltration, for the removal of color, turbidity, and other contaminants. The most common coagulants are iron salts (e.g., FeCl 6H O; FeCl ; FeSO 7H O; Fe (SO ) 7H O) and aluminum salts (e.g., 3· 2 2 4· 2 2 4 3· 2 Al (SO ) 18H O; AlCl ; Na Al O ). Aluminum salts are preferred for water treatment. They 2 4 3· 2 3 2 2 4 hydrolyze in water to aluminum hydroxide and then the colloidal and suspended contaminants are removed by charge neutralization, sweep ﬂoc mechanism, and adsorption onto hydroxide precipitates . Sludges generated from surface water treatments are called post-coagulation residuals and their composition depends on the coagulant used—iron (Fe-SWTRs) or aluminum (Al-SWTRs) . Al-SWTRs are composed mainly of aluminum oxide, whose content in the sludge varies in the range 14.5–46.0% [64–66]. A major component of Fe-SWTRs is iron oxide varying in weight fraction from 15.5% to 26% . Signiﬁcant amounts of SiO2 (26.2–41.8%) are also present in both types of SWTRs [55,64]. The content of organic substances can even reach 25% . The elemental composition of SWTRs is shown in Table2. The main elements of SWTRs generated during surface water treatment are Al and (some) Fe, which are components of coagulants . With an increase in the coagulant dosage, the amounts of Al and Fe also increase. A high organic carbon (C) content comes from organic compounds removed from the water or from activated carbon used for treatment [4,68]. Signiﬁcant concentrations of Ca, Mn, and Mg are also present as are heavy metals in low concentrations. For example, in the case of Al-SWTRs, concentrations of Cu, Zn, Cr, Cd, Pb, and As are 0.005–0.007, 0.009–0.011, 0.008–0.039, 0.001–0.028, 0.005–0.008, and 0.013–0.037 mg/L, respectively . Using WTRs as adsorbents, the materials should be considered as non-toxic wastes. As previous research shows, the release of metals from WTRs is negligible and therefore, they are non-toxic wastes [59,70]. Zhou and Haynes [68,69] also conducted leaching test. resulting in very low Cu, Zn, Cr, Cd, Pb, and As concentration in the leachate, below the respective USEPA (United States Environmental Protection Agency) regulatory guidelines for toxic wastes . Minerals 2019, 9, 487 5 of 17
Table 2. The concentration of selected elements in the post-coagulation water treatment residuals. (PAC—polyaluminum chloride, AC—activated carbon).
Chemical Composition Water Origin Water Treatment Process (mg/g) References Fe Al Ca Mn Mg C Fe and Al coagulation 71.2 62.7 18.9 2.9 2.4 -  Al coagulation 17.8 74.7 15.7 0.8 4.5 -  Al coagulation 23.9 122.0 0.4 - 0.2 103.0  Al coagulation + AC 17.2 73.5 0.4 - 1.8 346.0 Surface water Al coagulation 4.0 95.3 - - - 243.0  Fe coagulation 161.0 1.2 - - - 155.0 Al coagulation (PAC) 17.5 63.6 - 1.2 1.2 -  Al coagulation + AC (PAC) 11.5 53.3 - 1.4 2.3 - Aeration + pre-chlorination + Al Groundwater 26.0–90.0 105.0–144.0 3.2–3.6 0.03–1.1 0.2–2.3 -  coagulation + ﬁltration Minerals 2019, 9, 487 6 of 17
Scanning electron microscopy (SEM) analysis shows that Fe- and Al-SWTRs are heterogeneously mixed particles with irregular shapes and a variable pore diameter (0.6–4.3 nm), which prospectively
Mineralsguarantee 2019 a, 9 highly, x FOR reactivePEER REVIEW surface that favors the sorption [41,52]. X-ray diffraction (XRD) patterns6 showof 18 that post-coagulation residuals are amorphous and poorly ordered. However, some Fe-SWTR samples have peaks attributed to small amounts of crystalline Fe-(hydr)oxides . Analysis similarly shows that Al-SWTRsScanning contain electron quartz, calcite,microscopy feldspar, (SEM) and sometimes analysis illite shows/smectite that and Fe- kaolinite and asAl-SWTRs well . are heterogeneously mixed particles with irregular shapes and a variable pore diameter (0.6–4.3 nm), which3.2. Groundwater prospectively Treatment guarantee Residuals a highly reactive surface that favors the sorption [41,52]. X-ray diffractionIn most (XRD) cases, patterns groundwater show isthat treated post-coagula to removetion iron residuals and manganese. are amorph Thisous is and achieved poorly by ordered. aeration However,and ﬁltration some [54 ].Fe-SWTR The soluble samples Fe(II) have form ispeaks oxidized attributed to the insolubleto small Fe(III)amounts form of and crystalline the ﬂocs Fe-(hydr)oxidesare captured on . the Analysis ﬁlter bed similarly . Further shows oxidationthat Al-SWTRs of Fe andcontain Mn quartz, takes place calcite, in feldspar, the ﬁlter and bed, sometimesenhancing illite/smectite ﬁlter eﬀectiveness. and kaolinite As long as as well there . are no other pollutants in the water, no additional chemicals need to be used in this process [53,74–76]. The ﬁlters are periodically backwashed, and the 3.2.contaminants Groundwater retained Treatment in theResiduals ﬁlter bed during the water puriﬁcation process are washed away and collectedIn most in acases, clariﬁer. groundwater These pollutants is treated settle toand remo formve iron sediments and manganese. in the clariﬁer This and is achieved the resulting by aerationsludge is and known filtration as the .The residual soluble from deironing Fe(II) form and is demanganization oxidized to the insoluble of ground Fe(III) or inﬁltration form and water the flocs(Fe/Mn-GWTRs) are captured [74 on– 77the]. Thefilter main bed components. Further of oxidation Fe/Mn-GWTRs of Fe and are Mn iron takes and manganese place in the compounds, filter bed, enhancingespecially filter oxides effectiveness. [54,67]. Fe/ Mn-GWTRsAs long as there contain are ironno other oxides pollutants (24.3%), in manganese the water, oxides no additional (5.35%), chemicalsorganic carbon need to (5.3%), be used and in inorganic this process carbon [53,74–7 (0.73%)6]. The . filters are periodically backwashed, and the contaminantsFe, at a concentration retained in the of filter 300 mg bed/g, during is the mainthe water component purification of WTRs process generated are washed by groundwater away and collectedtreatment in processes a clarifier. [57 These]. A signiﬁcant pollutants amount settle and of Ca form is also sediments present. in The the concentration clarifier and ofthe these resulting metal sludgeions appears is known to be as inﬂuencedthe residual by from the qualitydeironing of rawand water.demanganization The WTRs also of ground contain or low infiltration concentrations water (Fe/Mn-GWTRs)of heavy metals [40[74–77].]. The main components of Fe/Mn-GWTRs are iron and manganese compounds,A typical especially SEM image oxides and [5 XRDpattern4,67]. Fe/Mn-GWTRs of WTRs contain are given iron in oxides Figure (24.3%),1. The samples manganese of GWTRs oxides (5.35%),reveal a organic typical microcrystalline-organogeniccarbon (5.3%), and inorganic microstructure,carbon (0.73%) with. small carbonate crystals embedded withinFe, substantialat a concentration cryptocrystalline of 300 mg/g, aggregated is the main iron component oxyhydroxides. of WTRs The generated particles by have groundwater irregular treatmentsurfaces with processes edges. . The residualsA significant are poorlyamount crystalline, of Ca is also just present. like Al/ Fe-GWTRs;The concentration however, of these the two-line metal ionsferrihydrite appears can to be be influenced noted. The by low-intensity the quality XRDof raw peaks water. are The indicative WTRs ofalso quartz contain and low calcite. concentrations All GWTRs ofpresented heavy metals in this . research [40,53,61] show a similar phase composition, indicating that sludge are rather amorphous material; the only crystalline mineral that was found was quartz .
Figure 1. Water treatment residuals (a) SEM image; (b) X-ray diﬀraction pattern (author’s materials). 3.3. Physicochemical Properties and Textural Parameters Figure 1. Water treatment residuals (a) SEM image; (b) X-ray diffraction pattern (author’s materials). Some properties of the residuals, such as textural parameters and chemical composition, inﬂuence the sorptionA typical capability. SEM image and XRDpattern of WTRs are given in Figure 1. The samples of GWTRs reveal a typical microcrystalline-organogenic microstructure, with small carbonate crystals embedded within substantial cryptocrystalline aggregated iron oxyhydroxides. The particles have irregular surfaces with edges. The residuals are poorly crystalline, just like Al/Fe-GWTRs; however, the two-line ferrihydrite can be noted. The low-intensity XRD peaks are indicative of quartz and calcite. All GWTRs presented in this research [40,53,61] show a similar phase composition, indicating that sludge are rather amorphous material; the only crystalline mineral that was found was quartz .
Minerals 2019, 9, 487 7 of 17
The residuals exhibit a wide range of speciﬁc surface area values, which depend on diﬀerent factors. As can be seen, typical surface water treatment residuals display relatively high speciﬁc surface areas in the range of 80 to 100 m2/g (Table3), when only Al and Fe salts are added. An addition of activated carbon increases the speciﬁc surface of the sludge. The particle size is extremely signiﬁcant for the speciﬁc surface area. Caporale et al.  noted that decreasing WTRs’ particle size in the range 1000–590 µm to below 125 µm increased the surface area of the sludge by almost 80% in the case of Fe-WTRs. Residuals from groundwater treatment displayed similar values of surface area: 120–170 m2/g.
Table 3. Comparison of some physical properties of WTRs (water treatment residuals). (PAC—polyaluminum chloride).
Water Origin Water Treatment Process Particle Size Speciﬁc Surface Area (m2/g) pH References Al & Fe coagulation <165 µm 81 7.6  Al coagulation <125 µm 97 6.8  Al coagulation + AC <125 µm 290 6.5 Al coagulation <125 µm 435 5.5 Surface water  Fe coagulation <125 µm 217 6.1 Al coagulation (PAC) <1 mm 50 5.6 Al coagulation + AC [53,73] <1 mm 413 5.6 (PAC) No reagents <1 mm 120 -  Groundwater No reagents <60 µm 152 7.0  No reagents <1 mm 170 - This study
The structure and chemical composition of, especially, the metal oxides in WTRs, because of their heterogenous nature with irregular shapes and a variable pore diameter, provide acceptable sorption properties. A key factor is that the residuals are dominated by amorphous oxides, which increase sorption capabilities in comparison to materials composed of more crystalline forms .
4.1. Adsorption Capacity of Post-Coagulation Residuals Ippolito et al.  showed that Al-SWTRs were a good selenium adsorbent. In 100 mL of 0.05 M NaCl solution, 2.5 g SWTRs was mixed with an appropriate amount of Na2SeO4 or Na2SeO3 to provide an Se(IV) and Se(VI) concentration of 60 mg/L. They stated that pH did not aﬀect the adsorption of selenate and selenite. Al-SWTRs adsorbed Se(VI) and Se(IV) in amounts of 1.4 to 2.1 mg/g and 1.4 to 1.95 m/g, respectively. Se(VI) adsorbed on the Al-SWTRs occurred as outer sphere complexes, while Se(IV) created inner-sphere complexation. The absence of inner-sphere complexation in case of Se(VI) implies that iron hydroxide impurities in Al-SWTRs have limited impact on Se(VI). In the 5–8 pH range, Se(IV) was reduced to Se(0). The adsorption was governed by the mixture of clay minerals and amorphous aluminum oxides. Siswoyo et al.  showed that SWTRs are a good cadmium(II) adsorbent. Diﬀerent doses of the adsorbent were added to 50 mL of Cd(II) solution at diﬀerent concentrations. The eﬀect of pH and time was evaluated. The maximum sorption capacities were 5.3 and 9.2 mg Cd/g, according to the Langmuir adsorption model. The SWTRs were strongly dependent on the pH of the solution. The removal eﬃciency of Cd(II) increased with the pH of the solution due to a decrease in H+ on the surface, which results in less repulsion with the metal ions . The favorable pH was in the range of 6.0 to 8.0. The amounts of adsorbed Cd(II) increased with an increase in the adsorbent dosage due to the greater accessibility of the surface area or binding sites [80,81]. The Cd(II) adsorption capacity Minerals 2019, 9, 487 8 of 17 increased rapidly for 30 min and then become constant until 24 h of shaking. The feasible mechanism of cadmium ion adsorption on STWRs is the ion exchange model . The capability of SWTRs for removing mercury was reported by Hovsepyan and Bonzongo . Commercial Hg(NO3)2 were used to prepare Hg(II) solutions with diﬀerent concentrations for batch sorption experiments. The solutions were kept in contact with dry Al-SWTRs in a 3:5 ratio. The maximum sorption capacity achieved was 79 mg Hg/g according to the Langmuir equation. Sorption isotherms indicated a strong aﬃnity of Hg(II) for Al-SWTRs. The highest Hg(II) removal eﬃciency was at pH 3.0 and the lowest at 5.0. The equilibrium was achieved in about 32 h. The best-ﬁt equation for sorption kinetic data was a pseudo-ﬁrst-order model, while use of the Weber–Morris and Bangham models indicated that the intraparticle diﬀusion might be the rate-limiting step for the Hg(II) immobilization on Al-SWTRs. The authors noted that further research concerning sorption mechanisms and the long-term stability of the created Hg with Al-SWTRs complexes is needed. Though several studies have demonstrated the ability of SWTRs to eﬃciently sorb metal ions from aqueous solutions, the mechanisms of metal sorption are still not fully understood. Quiñones et al.  carried out research on the sorption of mercury cations by Al-SWTRs and focused on the sorption mechanisms. They used a ﬂooding technique followed by wet and dry cycles to prepare Hg-spiked Al-SWTR samples. A known amount of Al-SWTRs is brought into contact with an HgCl2 solution at a 1:4 ratio. Three diﬀerent types of Al-SWTRs samples were prepared. Diﬀerent methods were used to determine the binding mechanisms of Hg(II) and Al-SWTRs. A signiﬁcant fraction of the added Hg was found to be locked in the residual fraction and was not mobile under natural environmental conditions. The organic Hg(II) fraction of Al-SWTRs, after the spiking and aging, was found to be prone to methylation by bacteria. However, there was signiﬁcant immobilization of Hg(II) by Al-SWTRs due to its binding to oxygen donor atoms of mineral ligands. Quiñones et al.  have also suggested that the use of additional methods, such as XANES (X-ray Absorption Near Edge Structure) and EXAFS (Extended X-ray Absorption Fine Structure), is necessary to explain the diﬀerent bonds between Hg(II) and electron donors more precisely. Jiao et al.  reported SWTRs as eﬀective cobalt(II) adsorbents. Batch adsorption experiments were carried out by agitating 0.5 g of SWTRs with 30 mL aqueous solution containing 0 to 800 mg/L of Co(II) on a shake table at a constant temperature of 25 ◦C. The sorption of Co(II) followed pseudo-second-order kinetics. Moreover, 90% of the equilibrium sorption capacity has been reached within the ﬁrst 12 h. The adsorption of Co(II) was a two-step process - quick adsorption of Co(II) on the external surface and possible slow intraparticle diﬀusion in the interior of the SWTR particles. The sorption isotherm was well-ﬁtted by the Langmuir model. The maximal adsorption capacity reached 17.307 mg/g. Co(II) removal was enhanced with increasing pH; this trend might be explained due to the changes in the surface charge characteristics of the SWTRs with pH . Adsorption is a spontaneous endothermic process. During desorption of Co(II), only minimal amount of compound was desorbed, and the process was strongly dependent on pH. Decreasing pH values might enhance Co(II) desorption. According to the FTIR analysis, the possible sorption mechanism is the formation of inner or outer sphere complexes between adsorbed Co(II) and the surface hydroxyl groups existing on the surface of the SWTRs. Zhou and Haynes  examined other Al-SWTRs for Pb(II), Cr(III), and Cr(VI) removal. Metal solutions of Pb(NO3)2, Cr(NO3)3, and Na2CrO4, with the desired metal concentration, were prepared in 0.01 M NaNO3 solution. A measured amount of sludge was weighed into 50 mL centrifuge tubes and 10 mL of 0.01 M NaNO3 was added. Adsorption capacity was highly dependent on the initial metal ion concentration, initial pH, and dosage. Adsorption of all compounds increased with an increasing equilibrium concentration of the adsorbate. Cr(III) and Pb(II) were preferably adsorbed at pH 6.0 to 9.0, which is typical for heavy metal cations , whereas Cr(VI) was adsorbed most eﬀectively at pH 2.0–4.0. It was found that equilibrium was reached in 120 min and 90% of maximum sorption had occurred. The higher the adsorbent dose was, the higher the amount of adsorbed metal ions due to an increase of the surface area and number of adsorption sites. Adsorption increased with an increasing Minerals 2019, 9, 487 9 of 17
temperature between 20 and 50 ◦C, suggesting that sorption is an endothermic process. The sorption isotherm was well ﬁtted to the Freundlich and Langmuir equations. The maximum adsorption capacities of Pb(II), Cr(III), and Cr(V) were 53.87–62.16 mg/g, 19.24–26.52 mg/g, and 10.92–11.44 mg/g, respectively. Kinetic data was correlated to a pseudo-second-order kinetic model for Cr(III) and Pb(II), implying that chemisorption was the rate-limiting step to sorption . Makris et al.  were one of the ﬁrst groups to deal with arsenic sorption onto Fe-SWTRs and Al-SWTRs. As sorption capacities of the WTRs were determined in batch equilibrium studies. Stock standard solutions were prepared in 0.01 M KCl. The pH was adjusted to 6.0. An initial screening study was performed to evaluate the eﬀectiveness of both SWTRs in removing As from the solution at a ﬁxed solid solution ratio (1:10). Detailed experiments were conducted to determine the eﬀect of the solid-solution ratio and time; pH was not controlled. Al-SWTRs sorbed greater amounts of As(V) than Fe-SWTRs (1.88–15 mg/g); however, As(III) was more preferably removed by Fe-SWTRs (7.5–15 mg/g). Al-SWTRs had greater sorption capabilities due to the higher speciﬁc surface area. Additional spectroscopic analysis should be conducted to explain the diﬀerences in As(III) and As(V) sorption. The sorption isotherm was well ﬁtted to the Freundlich equations. Sorption of As(III) and As(V) was a biphasic process. The beginning of the sorption was rapid; within the ﬁrst hour, 98% of the compound was removed, followed by a slower sorption rate. Kinetic data was correlated to a pseudo-second-order kinetic model. Zhou and Haynes  again examined Al-SWTRs for As(III), As(V), Se(IV), and Se(VI) removal. Metal solutions of NaAsO2, Na2HAsO4, Na2SeO3, and Na2SeO4 with the desired metal concentration were prepared in 0.01 M NaNO3. Materials and methodology were identical to those presented by Zhou and Haynes . Adsorption was strongly dependent on the pH. The adsorption decrease was rapid above pH 4.0 for Se(VI), above pH 5.0 for Se(IV), and above pH 6.0 for As(V). Adsorption of As(III) increased with increasing pH up to pH 9.0, then decreased. The sorption isotherm was well ﬁtted to the Freundlich and Langmuir equations. The As(III), As(V), Se(IV), and Se(VI) maximum adsorption capacities were 18.73, 20.98, 22.11, and 11.05 mg/g, respectively. Kinetic data were correlated to a pseudo-second-order kinetic model. The adsorption was rapid; equilibrium occurred after 120 min. Chemisorption was the rate-limiting step for adsorption. The study demonstrated that the metals were strongly bonded to the sludge surface and so they could not be easily leached from the material. Caporale et al.  reported another As-adsorbing Al-SWTRs and Fe-SWTRs. The authors investigated the eﬀect of the particle size of adsorbents on sorption. Four samples of Al-SWTRs and Fe-SWTRs with diﬀerent particle sizes were obtained. The solution volume was adjusted to 20 mL with 10 mmol/L KCl and the initial SWTRs-solution ratio was ﬁxed at 5 g/L. The eﬀects of pH (3.0–9.0) was investigated. The equilibrium data was well ﬁtted to the Langmuir equation. As(III) was more preferably sorbed than As(V) by Fe-WTRs, whereas As(V) was more willingly sorbed than As(III) by Al-SWTRs. Because of their higher surface area, the Al-SWTRs were more eﬀective sorbents. More eﬃcient removal of As was achieved by decreasing the SWTRs’ particle size. The speciﬁc surface area of the smallest particles of Fe-SWTRs and Al-SWTRs increased by 137 and 123 m2/g, respectively. The maximum adsorption capacities of Fe-SWTRs and Al-SWTRs with particle sizes <125 µm were 11.21 and 40.24 mg/g for As(III) and 9.19 and 49.98 mg/g for As(V). However, the eﬀect of the particle size was more evident in the case of Fe-SWTRs than Al-SWTRs. It might be caused by a large increase in the surface area of SWTRs containing Fe corresponding to the decrease in particle size. The highest sorption of As(III) and As(V) by Al-SWTRs was noted at pH 6.0 to 7.0, whereas the adsorption capacity of Fe-SWTRs seemed to be independent of pH. Other As(V) adsorbing SWTRs were reported by Elkhatib et al. . They synthesized WTRs on a nanoscale (nSWTRs), with particle sizes <100 nm. Adsorption studies were conducted at pH 7.2 and the eﬀect of pH, time, dosage of nSWTRs, and the initial concentration was determined. As(V) adsorption was highest at pH 3 (88%) and the least at pH 11 (14.9%), due to the increase in the coulomb repulsive force between the surface of SWTRs and As(V) as the solution pH increases . The equilibrium data was well-ﬁtted to the Langmuir and Temkin models. Adsorption of As(V) was Minerals 2019, 9, 487 10 of 17 biphasic, consisting of a rapid sorption followed by much slower sorption phase. The maximum As(V) sorption capacity reached was 50 mg/g. nSWTRs achieved a higher maximum sorption capacity than µWTRs (<51 µm) and mWTRs (2 mm). A possible mechanism for As(V) sorption was the formation of bidentate (adsorption of arsenate ions onto iron hydroxides) and monodentate (adsorption of As(V) onto aluminum hydroxides) surface complexes. The power function model best described As(V) adsorption on nSWTRs. The results of the desorption process point to the stability of As-SWTRs surface complexes.
4.2. Adsorption Capacity of Groundwater Treatment Residual Wu et al.  reported the possible usage of Fe-based backwashed sludge for arsenite removal from water. In the sorption study, 0.06 g of GWTRs was added to 100 mL of As(III) solution with diﬀerent initial concentrations. The maximum adsorption of As(III) reached was 59.7 mg/g, according to the Langmuir model. The As(III) removal eﬃciency was strongly dependent on the solution pH, with the best results obtained for pH 8.0. The subsequent increase of pH led to decrease of sorption eﬀectiveness due. It could be assigned to the electrical repulsion between GWTRs and As(III) anions . Higher adsorbent dosages resulted in higher As(III) removal eﬃciency. The removal of As(III) increased rapidly in the ﬁrst 1 h, however, equilibrium adsorption was reached after 18 h. The kinetic data correlated with both the Elovich model and the power model. Adsorption was an endothermic process, which is in line with other researches [41,69]. The removal of As(III) by GWTRs was mainly controlled by adhesion and ligand exchange between the As species and sulfate. Desorption results show that As(III) may be released only at strong alkali metals or high phosphate concentrations. Oci´nskiet al.  studied the As(III) and As(V) adsorption properties of the WTRs generated during the deironing and demanganization processes of inﬁltration water. Adsorption studies were carried out in a batch regime. As solutions were brought in contact with the GWTR powder in a 100 or 250 cm3 conical ﬂask. The eﬀect of pH, initial concentration of As(III) and As(V), and time was evaluated. The maximum adsorption capacity determined by the Langmuir isotherm equations reached 132 mg/g for As(III) and 77 mg/g for As(V). The explanation of this trend is the oxidation of As(III) to As(V) accompanied with reductive dissolution of iron and manganese oxides. A signiﬁcant factor for the sorption process is the presence of iron oxyhydroxides and humic substances in the residuals. The As(III) and As(V) removal eﬃciency was strongly dependent on the solution pH, with the best results obtained at pH 4.0, and a slight decrease in adsorption observed at pH 10.0. The removal of arsenic species was a rapid process and 90 min was required to remove 80% of the contaminant. Kinetic studies revealed two-step chemisorption of inner-sphere As(III) complexes. As(V) adsorption was controlled by external and intraparticle diﬀusion. Attempts were made to regenerate the GWTRs, but the values of desorption were low. Ong et al.  evaluated the nickel ion adsorption capability of GWTRs. The eﬀects of varying solution pH, initial nickel concentration, and contact time were investigated. The results showed that the pH (4.5 to 7.5) had no inﬂuence on Ni(II) removal. The maximum sorption capacity was 11.6 mg/g. The sorption isotherm was well-ﬁtted to Freundlich equations. Sorption capacity increased with an increasing initial concentration. The equilibrium was achieved after 120 min. Sorption kinetic data was best-ﬁtted to a pseudo-second-order adsorption kinetic model, indicating that chemisorption which is associated with the formation of a covalent bond through the exchange or sharing of electrons between metal ions and the binding sites of the adsorbent, was the dominant process . We also conducted similar research, including batch sorption experiments of selected heavy metals and metalloids. The details concerning the methodology of the sorption experiments are in Section 2.2. The maximum amounts of removed Cr(III), Cr(VI), As(V), Cd(II), Pb(II), Zn(II), and Cu(II) were 22.3, 51.3, 24.8, 4.8, 92.7, 19.2, and 31.2 mg/g, respectively. The removal eﬃciency was strongly dependent on the initial metal concentration, which is a common trend in all presented researches. The sorption eﬃciency at the initial concentration of 100 mM/L was on average, 300 to 500 times higher than at a concentration of 0.1 mM/L. Cd(II) was the least adsorbed compound, while Pb(II) was the Minerals 2019, 9, 487 11 of 17 best adsorbed. Due to the relatively high adsorption capacity of GWTRs toward all heavy metals and metalloids, the aim of further studies will be to measure the eﬀect of pH, temperature, and time of reaction on sorption capacity.
5. Discussion Table4 shows the comparison of the speciﬁc surface area of all WTRs that are described in this paper, as well as their favorable adsorption test conditions. It is evident that sorption capacity depends on many diﬀerent factors, such as the nature of sorbent surface, the properties of the sorbents, and the experimental conditions. WTRs create particles with irregular surfaces and edges, which provide WTRs with a highly reactive surface for sorption metals . Sorption capacity also depends on the particle size of WTRs. The smaller particle size and therefore the higher surface area and the greater amounts of heavy metals and metalloids being sorbed. This trend was caused by an increasing surface area. Therefore, it is impossible to compare all these results, as the presented researches diﬀer in sorption conditions and methodology. As the results [4,40,61,68,87] showed, GWTRs exhibited better sorption capacity for As(III) and As(V) than SWTRs. The reason might be a higher concentration of iron and manganese oxides as well as a well-developed speciﬁc surface area [40,91]. However, in case of SWTRs, Al-SWTRs samples sorbed greater amounts of As(III) and As(V) than Fe-SWTRs. It might be explained by a higher surface area and higher organic matter content in Al-SWTRs. Fe-SWTRs was better sorbent in the case of As(III) than As(V), whereas more As(V) was sorbed by Al-SWTRs [4,87]. Se(IV), Se(VI), Cr(III), and Cr(VI) were removed in similar amounts. Among the cations, Hg(II) and Pb(II) were best sorbed, and Cd(II) and Ni(II) the least. However, the reason may be simply diﬀerent sorption coditions. In most cases, sorption processes were dependent on pH and the best results were obtained for pH 6.0 to 7.0. Adsorption of the metal cations, (Pb(II), Cd(II), Co(II), and Ni(II)), on WTRs depends on pH, with an increasing pH of the solution the removal eﬃciency was higher [41,69,73,89]. It might be explained by the fact that metal ions form complexes with acidic functional groups in the sorbent . In case of decreasing pH, protons compete with metal ions for the binding sites on the WTRs surface and the protons decrease the negative charges [73,79]. In case of anions, the lower pH favored the sorption capacity . However, as Wu et al.  noted As(III) was favorably sorbed with pH 8.0. The further increase of the pH led to a decrease of As(III) removal and it could be attributed to the electrical repulsion force between GWTRs and As(III) anions. The most common sorption mechanism of metals and metalloids on WTRs was chemisorption, which involves an exchange between metal anions/cations and surface ligands and the formation of a covalent with the surface . In most references, the sorption kinetic increased up to 120 min of experiments then decreased. Sorption of the described metals and metalloids was biphasic. The immediate sorption phase was followed by a much slower sorption phase. The rapid sorption might be due to the availability of active adsorption sites . In almost all experiments, sorption capacity increased with an increase in the initial pollutant concentration. The sorption eﬃciency increased with increasing doses of adsorbent. This is assigned to the increasing surface area and number of adsorption sites with an increasing dose . Temperatures were in the range of 23 to 25 ◦C, showing that the processes had been carried out at room temperature. However, sometimes the sorption process was more eﬃcient in a higher temperature (20–50 ◦C), suggesting that sorption onto WTRs’ surface is an endothermic process. This trend is noted for speciﬁcally adsorbing ions, which result in activation of the adsorbent surface [69,93]. Desorption has not been successful, only low values of contaminants were desorbed, and waste can be safely stored. For example, As(III) may be released only at strong alkali or high phosphate concentrations . Minerals 2019, 9, 487 12 of 17
Table 4. Main characteristics and uptake capacities of WTRs for heavy metals and metalloids removal (SSA—speciﬁc surface area).
Adsorbent Favorable Adsorption Test Conditions SSA Initial Concentration Temp. Contact Time Adsorption Capacity Reference Type 2 Heavy Metals to be Removed pH (m /g) (mg/L) (◦C) (min) (mg/g) 217.4 80 7.0–9.0 - 24 h 11.2  Fe-SWTRs - 200 - 23 60 14.5  152 120 8.0 25 60 59.7  Fe-GWTRs 120As(III) 25 4.0 - 90 132.0  435.5 105 6.0–7.0 - 24 h 40.2  Al-SWTRs - 200 - 23 60 9.0  97.3 74 9.0 25 120 18.73  217.4 80 - - 24 h 9.2  Fe-SWTRs - 200 - 23 60 10.0  Fe-GWTRs 120 25 4.0 - 90 77.0  435.5As(V) 105 - - 24 h 49.9  - 200 - 23 60 15.0  97.3 74 6.0 25 120 20.98  - 160 5.0–7.0 23 15 50.0  97.3 Cr(III) 52 6.0–9.0 25 120 19.2  97.3 Cr(VI) 52 2.0–4.0 25 120 10.9 Al-SWTRs 97.3 79 5.0 25 120 22.11  Se(IV) 50 60 6.0–8.0 25 24 h 2.1  97.3 79 4.0 25 120 11.05  Se(VI) 50 60 6.0–8.0 25 24 h 1.9  97.3 Pb(II) 207 6.0–9.0 25 120 53.9  - Hg(II) 40 3.0 - 32 h 79.0  50 Cd(II) 100 6.0–8.0 - 30 5.3  Fe/Al-SWTRs 81.0 Co(II) 800 8.0 25 12 h 17.3  GWTRs - Ni(II) 200 6.5 25 120 11.6  Minerals 2019, 9, 487 13 of 17
6. Conclusions The pollution of surface and groundwater with heavy metals is a major issue worldwide, and the development of suitable technology to remove heavy metals from the aqueous solutions is necessary. WTRs have a surprisingly good sorption capacity for diﬀerent compounds, especially heavy metals and metalloids. The comparisons of sorption properties of various WTRs is diﬃcult because of incoherence in the data, such as diﬀerent chemical compositions of the treated water, various coagulants used, sorbent preparation, and testing methods. However, in most studies, the sorption eﬃciency was dependent on the pH of the solution, reaction time, temperature, and initial metal concentration in the solution. Decrease in particles size enhanced sorption properties due to increases in the speciﬁc surface area. The presence of iron and/or aluminum oxides was an important factor in the sorption process. WTRs are waste materials that can be used as low-cost, safe, and eﬀective adsorbents for the removal of heavy metal cations and anions from polluted water. GWTRs, containing high iron and manganese oxides can be used to remove arsenic. As almost all of the publications presented above have proven, there are still many gaps in the knowledge about WTRs and their sorption properties. More research is required on the sorption mechanism, the desorption process as well as the long-term stability of formed metal–WTRs complexes. Sorption experiments of mixtures of selected compounds need to be carried out.
Author Contributions: T.B. designed and supervised the project; M.W. performed part of the experiments from this review, analyzed the data, and wrote this paper. T.B., M.K.-K., A.P., and G.R. submitted comments and corrected it. Funding: This research was funded by the National Science Centre, Poland Grant No. 2017/27/N/ST10/00713 and PUT research project 01/13/DSPB/0891. Conﬂicts of Interest: The authors declare no conﬂict of interest. The funders had no role in the design of the study; in the collection, analyses or interpretation of data; in the writing of the manuscript and in the decision to publish the results.
1. Salem, H.M.; Eweida, E.A.; Farag, A. Heavy metals in drinking water and their environmental impact of human health. In Proceedings of the International Conference for Environmental Hazards Mitigation, Cairo, Egypt, 9–12 September 2000; pp. 542–556. 2. Burakov, A.E.; Galunin, E.V.; Burakova, I.V.; Kucherova, A.E.; Agarwal, S.; Tkachev, A.G.; Gupta, V.K. Adsorption of heavy metals on conventional and nanostructured materials for wastewater treatment purposes: A review. Ecotoxicol. Environ. Saf. 2018, 148, 702–712. [CrossRef][PubMed] 3. Elkhatib, E.; Mahdy, A.; Sherif, F.; Hamadeen, H. Evaluation of a Novel Water Treatment Residual Nanoparticles as a Sorbent for Arsenic Removal. J. Nanomater. 2015, 2015, 10. [CrossRef] 4. Caporale, A.G.; Punamiya, P.; Pigna, M.; Violante, A.; Sarkar, D. Eﬀect of particle size of drinking-water treatment residuals on the sorption of arsenic in the presence of competing ions. J. Hazard. Mater. 2013, 260, 644–651. [CrossRef][PubMed] 5. Chen, Y.-Y.; Yu, S.-H.; Jiang, H.-F.; Yao, Q.-Z.; Fu, S.-Q.; Zhou, G.-T. Performance and mechanism of simultaneous removal of Cd(II) and Congo red from aqueous solution by hierarchical vaterite spherulites. Appl. Surf. Sci. 2018, 444, 224–234. [CrossRef] 6. Cao, W.; Wang, Z.; Ao, H.; Yuan, B. Removal of Cr(VI) by corn stalk based anion exchanger: The extent and rate of Cr(VI) reduction as side reaction. Colloids Surf. A Physicochem. Eng. Asp. 2018, 539, 424–432. [CrossRef] 7. Dinari, M.; Haghighi, A. Ultrasound-assisted synthesis of nanocomposites based on aromatic polyamide and modiﬁed ZnO nanoparticle for removal of toxic Cr(VI) from water. Ultrason. Sonochem. 2018, 41, 75–84. [CrossRef][PubMed] 8. Lingamdinne, L.P.; Koduru, J.R.; Roh, H.; Choi, Y.-L.; Chang, Y.-Y.; Yang, J.-K. Adsorption removal of Co(II) from waste-water using graphene oxide. Hydrometallurgy 2016, 165, 90–96. [CrossRef] 9. Hu, H.M.; Li, X.W.; Huang, P.W.; Zhang, Q.W.; Yuan, W.Y. Eﬃcient removal of copper from wastewater by using mechanically activated calcium carbonate. J. Environ. Manag. 2017, 203, 1–7. [CrossRef][PubMed] Minerals 2019, 9, 487 14 of 17
10. Khatri, N.; Tyagi, S.; Rawtani, D. Recent strategies for the removal of iron from water: A review. J. Water Process. Eng. 2017, 19, 291–304. [CrossRef] 11. Liu, J.; Mwamulima, T.; Wang, Y.; Fang, Y.; Song, S.; Peng, C. Removal of Pb(II) and Cr(VI) from aqueous solutions using the ﬂy ash-based adsorbent material-supported zero-valent iron. J. Mol. Liq. 2017, 243, 205–211. [CrossRef] 12. Dubey, R.; Bajpai, J.; Bajpai, A. Chitosan-alginate nanoparticles (CANPs) as potential nanosorbent for removal of Hg (II) ions. Environ. Nanotechnol. Monit. Manag. 2016, 6, 32–44. [CrossRef] 13. Ali, I. The Quest for Active Carbon Adsorbent Substitutes: Inexpensive Adsorbents for Toxic Metal Ions Removal from Wastewater. Sep. Purif. Rev. 2010, 39, 95–171. [CrossRef] 14. Zhang, X.T.; Wang, X.M. Adsorption and Desorption of Nickel(II) Ions from Aqueous Solution by a Lignocellulose/Montmorillonite Nanocomposite. PLoS ONE 2015, 10, e0117077. [CrossRef] 15. Hoseinian, F.S.; Rezai, B.; Kowsari, E.; Safari, M. Kinetic study of Ni(II) removal using ion ﬂotation: Eﬀect of chemical interactions. Miner. Eng. 2018, 119, 212–221. [CrossRef] 16. Omraei, M.; Esfandian, H.; Katal, R.; Ghorbani, M. Study of the removal of Zn(II) from aqueous solution using polypyrrole nanocomposite. Desalination 2011, 271, 248–256. [CrossRef] 17. Fu, F.; Wang, Q. Removal of heavy metal ions from wastewaters: A review. J. Environ. Manag. 2011, 92, 407–418. [CrossRef] 18. Mauchauﬀée, S.; Meux, E. Use of sodium decanoate for selective precipitation of metals contained in industrial wastewater. Chemosphere 2007, 69, 763–768. [CrossRef] 19. Verma, V.; Tewari, S.; Rai, J. Ion exchange during heavy metal bio-sorption from aqueous solution by dried biomass of macrophytes. Bioresour. Technol. 2008, 99, 1932–1938. [CrossRef] 20. Lai, Y.-C.; Chang, Y.-R.; Chen, M.-L.; Lo, Y.-K.; Lai, J.-Y.; Lee, D.-J. Poly(vinyl alcohol) and alginate cross-linked matrix with immobilized Prussian blue and ion exchange resin for cesium removal from waters. Bioresour. Technol. 2016, 214, 192–198. [CrossRef] 21. Cochrane, E.; Lu, S.; Gibb, S.; Villaescusa, I.; Gibb, S. A comparison of low-cost biosorbents and commercial sorbents for the removal of copper from aqueous media. J. Hazard. Mater. 2006, 137, 198–206. [CrossRef] 22. Davarnejad, R.; Panahi, P. Cu (II) removal from aqueous wastewaters by adsorption on the modiﬁed Henna
with Fe3O4 nanoparticles using response surface methodology. Sep. Purif. Technol. 2016, 158, 286–292. [CrossRef] 23. Landaburu-Aguirre, J.; Pongracz, E.; Peramaki, P.; Keiski, R.L. Micellar-enhanced ultraﬁltration for the removal of cadmium and zinc: Use of response surface methodology to improve understanding of process performance and optimisation. J. Hazard. Mater. 2010, 180, 524–534. [CrossRef] 24. Rahmanian, B.; Pakizeh, M.; Esfandyari, M.; Heshmatnezhad, F.; Maskooki, A. Fuzzy modeling and simulation for lead removal using micellar-enhanced ultraﬁltration (MEUF). J. Hazard. Mater. 2011, 192, 585–592. [CrossRef] 25. Mohsen-Nia, M.; Montazeri, P.; Modarress, H. Removal of Cu2+ and Ni2+ from wastewater with a chelating agent and reverse osmosis processes. Desalination 2007, 217, 276–281. [CrossRef] 26. Yoon, J.; Amy,G.; Chung, J.; Sohn, J.; Yoon, Y.Removal of toxic ions (chromate, arsenate, and perchlorate) using reverse osmosis, nanoﬁltration, and ultraﬁltration membranes. Chemosphere 2009, 77, 228–235. [CrossRef] 27. Lertlapwasin, R.; Bhawawet, N.; Imyim, A.; Fuangswasdi, S. Ionic liquid extraction of heavy metal ions by 2-aminothiophenol in 1-butyl-3-methylimidazolium hexaﬂuorophosphate and their association constants. Sep. Purif. Technol. 2010, 72, 70–76. [CrossRef] 28. Akbal, F.; Camci, S. Copper, chromium and nickel removal from metal plating wastewater by electrocoagulation. Desalination 2011, 269, 214–222. [CrossRef] 29. Dharnaik, A.S.; Ghosh, P.K. Hexavalent chromium Cr(VI) removal by the electrochemical ion-exchange process. Environ. Technol. 2014, 35, 2272–2279. [CrossRef] 30. Lee, C.G.; Jeon, J.W.; Hwang, M.J.; Ahn, K.H.; Park, C.; Choi, J.W.; Lee, S.H. Lead and copper removal from aqueous solutions using carbon foam derived from phenol resin. Chemosphere 2015, 130, 59–65. [CrossRef] 31. Maneechakr, P.; Karnjanakom, S. Adsorption behaviour of Fe(II) and Cr(VI) on activated carbon: Surface chemistry, isotherm, kinetic and thermodynamic studies. J. Chem. Thermodyn. 2017, 106, 104–112. [CrossRef] 32. Petrus, R.; Warchol, J.K. Heavy metal removal by clinoptilolite. An equilibrium study in multi-component systems. Water Res. 2005, 39, 819–830. [CrossRef] Minerals 2019, 9, 487 15 of 17
33. Bajda, T.; Klapyta, Z. Adsorption of chromate from aqueous solutions by HDTMA-modiﬁed clinoptilolite, glauconite and montmorillonite. Appl. Clay Sci. 2013, 86, 169–173. [CrossRef] 34. Bajda, T.; Szala, B.; Solecka, U. Removal of lead and phosphate ions from aqueous solutions by organo-smectite. Environ. Technol. 2015, 36, 2872–2883. [CrossRef] 35. He, Y.; Liu, Q.Q.; Hu, J.; Zhao, C.X.; Peng, C.J.; Yang, Q.; Wang, H.L.; Liu, H.L. Eﬃcient removal of Pb(II) by amine functionalized porous organic polymer through post-synthetic modiﬁcation. Sep. Purif. Technol. 2017, 180, 142–148. [CrossRef] 36. Wang, Y.Y.; Liu, Y.X.; Lu, H.H.; Yang, R.Q.; Yang, S.M. Competitive adsorption of Pb(II), Cu(II), and Zn(II) ions onto hydroxyapatite-biochar nanocomposite in aqueous solutions. J. Solid State Chem. 2018, 261, 53–61. [CrossRef] 37. Chen, J.G.; Kong, H.N.; Wu, D.Y.; Chen, X.C.; Zhang, D.L.; Sun, Z.H. Phosphate immobilization from aqueous solution by ﬂy ashes in relation to their composition. J. Hazard. Mater. 2007, 139, 293–300. [CrossRef] 38. Lim, J.W.; Chang, Y.Y.; Yang, J.K.; Lee, S.M. Adsorption of arsenic on the reused sanding wastes calcined at diﬀerent temperatures. Colloids Surf. A Physicochem. Eng. Asp. 2009, 345, 65–70. [CrossRef] 39. Lingamdinne, L.P.; Yang, J.K.; Chang, Y.Y.; Koduru, J.R. Low-cost magnetized Lonicera japonica ﬂower biomass for the sorption removal of heavy metals. Hydrometallurgy 2016, 165, 81–89. [CrossRef] 40. Ocinski, D.; Jacukowicz-Sobala, I.; Mazur, P.; Raczyk, J.; Kociolek-Balawejder, E. Water treatment residuals containing iron and manganese oxides for arsenic removal from water—Characterization of physicochemical properties and adsorption studies. Chem. Eng. J. 2016, 294, 210–221. [CrossRef] 41. Jiao, J.; Zhao, J.B.; Pei, Y.S. Adsorption of Co(II) from aqueous solutions by water treatment residuals. J. Environ. Sci. 2017, 52, 232–239. [CrossRef] 42. Rzepa, G.; Bajda, T.; Ratajczak, T. Utilization of bog iron ores as sorbents of heavy metals. J. Hazard. Mater. 2009, 162, 1007–1013. [CrossRef] 43. Jia, Y.F.; Demopoulos, G.P. Adsorption of arsenate onto ferrihydrite from aqueous solution: Inﬂuence of media (sulfate vs nitrate), added gypsum, and pH alteration. Environ. Sci. Technol. 2005, 39, 9523–9527. [CrossRef] 44. Gao, Y.; Mucci, A. Individual and competitive adsorption of phosphate and arsenate on goethite in artiﬁcial seawater. Chem. Geol. 2003, 199, 91–109. [CrossRef] 45. Violante, A.; Pucci, M.; Cozzolino, V.; Zhu, J.; Pigna, M. Sorption/desorption of arsenate on/from Mg-Al layered double hydroxides: Inﬂuence of phosphate. J. Colloid Interface Sci. 2009, 333, 63–70. [CrossRef] 46. Xie, J.K.; Xu, H.M.; Qu, Z.; Huang, W.J.; Chen, W.M.; Ma, Y.P.; Zhao, S.J.; Liu, P.; Yan, N.Q. Sn-Mn binary metal oxides as non-carbon sorbent for mercury removal in a wide-temperature window. J. Colloid Interface Sci. 2014, 428, 121–127. [CrossRef] 47. Zhang, W.; Liu, C.H.; Zheng, T.; Ma, J.; Zhang, G.S.; Ren, G.H.; Wang, L.; Liu, Y.L. Eﬃcient oxidation and sorption of arsenite using a novel titanium (IV)-manganese(IV) binary oxide sorbent. J. Hazard. Mater. 2018, 353, 410–420. [CrossRef] 48. Mikhaylov, V.I.; Maslennikova, T.P.; Krivoshapkina, E.F.; Tropnikov, E.M.; Krivoshapkin, P.V. Express Al/Fe oxide-oxyhydroxide sorbent systems for Cr(VI) removal from aqueous solutions. Chem. Eng. J. 2018, 350, 344–355. [CrossRef] 49. Altundogan, H.S.; Altundogan, S.; Tumen, F.; Bildik, M. Arsenic adsorption from aqueous solutions by activated red mud. Waste Manag. 2002, 22, 357–363. [CrossRef] 50. Evuti, A.M.; Lawal, M. Recovery of coagulants from water works sludge: A review. Adv. Appl. Sci. Res. 2011, 2, 410–417. 51. Magdalena, W.; Tomasz, B. Current stage of knowledge relating to the use of ferruginous sludge from water treatment plants—A preliminary review of the literature. Mineralogia 2017, 48, 9–45. 52. Quinones, K.D.; Hovsepyan, A.; Oppong-Anane, A.; Bonzongo, J.C.J. Insights into the mechanisms of mercury sorption onto aluminum based drinking water treatment residuals. J. Hazard. Mater. 2016, 307, 184–192. [CrossRef] 53. Wołowiec, M.; Pruss, A.; Komorowska-Kaufman, M.; Lasocka-Gomuła, I.; Rzepa, G.; Bajda, T. The properties of sludge formed as a result of coagulation of backwash water from ﬁlters removing iron and manganese from groundwater. SN Appl. Sci. 2019, 1, 639. [CrossRef] Minerals 2019, 9, 487 16 of 17
54. Komorowska-Kaufman, M. Adsorption properties of sludge arising during processes of groundwater and surface water treatment—A review. In Sorbenty Mineralne—Surowce, Energetyka, Ochrona Srodowiska,´ Nowoczesne Technologie; Bajda, T., Ed.; Wydawnictwo Naukowe AGH: Kraków, Polska, 2017; pp. 65–75. 55. Babatunde, A.O.; Zhao, Y.Q. Constructive approaches toward water treatment works sludge management: An international review of beneﬁcial reuses. Crit. Rev. Environ. Sci. Technol. 2007, 37, 129–164. [CrossRef] 56. Yang, L.; Wei, J.; Zhang, Y.M.; Wang, J.L.; Wang, D.T. Reuse of acid coagulant-recovered drinking waterworks sludge residual to remove phosphorus from wastewater. Appl. Surf. Sci. 2014, 305, 337–346. [CrossRef] 57. Krishna, K.C.B.; Aryal, A.; Jansen, T. Comparative study of ground water treatment plants sludges to remove phosphorous from wastewater. J. Environ. Manag. 2016, 180, 17–23. [CrossRef] 58. Makris, K.C.; Harris, W.G.; O’Connor, G.A.; Obreza, T.A. Phosphorus immobilization in micropores of drinking-water treatment residuals: Implications for long-term stability. Environ. Sci. Technol. 2004, 38, 6590–6596. [CrossRef] 59. Hovsepyan, A.; Bonzongo, J.C.J. Aluminum drinking water treatment residuals (Al-WTRs) as sorbent for mercury: Implications for soil remediation. J. Hazard. Mater. 2009, 164, 73–80. [CrossRef] 60. Gibbons, M.K.; Gagnon, G.A. Understanding removal of phosphate or arsenate onto water treatment residual solids. J. Hazard. Mater. 2011, 186, 1916–1923. [CrossRef] 61. Wu, K.; Liu, R.P.; Li, T.; Liu, H.J.; Peng, J.M.; Qu, J.H. Removal of arsenic(III) from aqueous solution using a low-cost by-product in Fe-removal plants-Fe-based backwashing sludge. Chem. Eng. J. 2013, 226, 393–401. [CrossRef] 62. Sales, A.; de Souza, F.R.; Almeida, F.D.R. Mechanical properties of concrete produced with a composite of water treatment sludge and sawdust. Constr. Build. Mater. 2011, 25, 2793–2798. [CrossRef] 63. Ahmad, T.; Ahmad, K.; Ahad, A.; Alam, M. Characterization of water treatment sludge and its reuse as coagulant. J. Environ. Manag. 2016, 182, 606–611. [CrossRef] 64. Vinitnantharat, S.; Kositchaiyong, S.; Chiarakorn, S. Removal of ﬂuoride in aqueous solution by adsorption on acid activated water treatment sludge. Appl. Surf. Sci. 2010, 256, 5458–5462. [CrossRef] 65. Yang, Y.; Tomlinson, D.; Kennedy, S.; Zhao, Y.Q. Dewatered alum sludge: A potential adsorbent for phosphorus removal. Water Sci. Technol. 2006, 54, 207–213. [CrossRef] 66. Kyncl, M.; Cˇ íhalová, Š.; Jurokova,ˇ M.; Langarová, S. Disposal and reuse of the water processing sludge. In˙z.Miner. 2012, 2, 11–20. 67. Szerzyna, S. Porcjowe Grawitacyjne Zag˛eszczenieOsadów Powstaj ˛acychW Ró˙znychUkładach Oczyszczania Wody; Politechnika Wrocławska: Wrocław, Polska, 2012. 68. Zhou, Y.F.; Haynes, R.J. A Comparison of Water Treatment Sludge and Red Mud as Adsorbents of As and Se in Aqueous Solution and Their Capacity for Desorption and Regeneration. Water Air Soil Pollut. 2012, 223, 5563–5573. [CrossRef] 69. Zhou, Y.F.; Haynes, R.J. Removal of Pb(II), Cr(III) and Cr(VI) from Aqueous Solutions Using Alum-Derived Water Treatment Sludge. Water Air Soil Pollut. 2011, 215, 631–643. [CrossRef] 70. Wang, C.H.; Yuan, N.N.; Pei, Y.S. Eﬀect of pH on Metal Lability in Drinking Water Treatment Residuals. J. Environ. Qual. 2014, 43, 389–397. [CrossRef] 71. USEPA. The Toxicity Characteristic Leaching Procedure; USEPA: Washington, DC, USA, 1992. 72. Ippolito, J.A.; Scheckel, K.G.; Barbarick, K.A. Selenium adsorption to aluminum-based water treatment residuals. J. Colloid Interface Sci. 2009, 338, 48–55. [CrossRef] 73. Siswoyo, E.; Mihara, Y.; Tanaka, S. Determination of key components and adsorption capacity of a low cost adsorbent based on sludge of drinking water treatment plant to adsorb cadmium ion in water. Appl. Clay Sci. 2014, 97-98, 146–152. [CrossRef] 74. Postawa, A. Best Practice Guide on the Control of Iron and Manganese in Water Supply; Hayes, C., Ed.; IWA Publishing: London, UK, 2013; p. 131. 75. Pruss, A.; Je˙z-Walkowiak, J.; Soza´nski,M.M. Concentration of heavy metals on surface of ﬁlter materials and in backwash water. In Metals and Related Substances in Drinking Water, COST Action 637, Proceedings of the 4th International Conference of METEAU, Kristianstad, Sweden, 13–15 October 2010; IWA Publishing: London, UK, 2011; pp. 217–222. Minerals 2019, 9, 487 17 of 17
76. Jez-Walkowiak, J.; Pruss, A.; Soza´nski,M.M. Applied technologies and possibilities of modernization of groundwater treatment plants in Poland. In Metals and Related Substances in Drinking Water, COST Action 637, Proceedings of the 4th International Conference of METEAU, Kristianstad, Sweden, 13–15 October 2010; IWA Publishing: London, UK, 2011; pp. 172–175. 77. Pruss, A.; Pruss, P.; Jedrzejczak, A. Hydraulic losses generated by modern drainage systems during backwash of rapid ﬁlters. Ochr. Sr.´ 2011, 33, 47–48. 78. Dixit, S.; Hering, J.G. Comparison of arsenic(V) and arsenic(III) sorption onto iron oxide minerals: Implications for arsenic mobility. Environ. Sci. Technol. 2003, 37, 4182–4189. [CrossRef] 79. Kadirvelu, K.; Namasivayam, C. Activated carbon from coconut coirpith as metal adsorbent: Adsorption of Cd(II) from aqueous solution. Adv. Environ. Res. 2004, 8, 729. [CrossRef] 80. Rao, M.M.; Ramesh, A.; Rao, G.P.C.; Seshaiah, K. Removal of copper and cadmium from the aqueous solutions by activated carbon derived from Ceiba pentandra hulls. J. Hazard. Mater. 2006, 129, 123–129. [CrossRef] 81. Wang, Y.; Tang, X.W.; Chen, Y.M.; Zhan, L.T.; Li, Z.Z.; Tang, Q. Adsorption behavior and mechanism of Cd(II) on loess soil from China. J. Hazard. Mater. 2009, 172, 30–37. [CrossRef] 82. Gupta, V.K.; Jain, C.K.; Ali, I.; Sharma, M.; Saini, V.K. Removal of cadmium and nickel from wastewater using bagasse ﬂy ash—A sugar industry waste. Water Res. 2003, 37, 4038–4044. [CrossRef] 83. Axe, L.; Trivedi, P. Intraparticle surface diﬀusion of metal contaminants and their attenuation in microporous amorphous Al, Fe, and Mn oxides. J. Colloid Interface Sci. 2002, 247, 259–265. [CrossRef] 84. Wang, C.H.; Guo, W.; Tian, B.H.; Pei, Y.S.; Zhang, K.J. Characteristics and kinetics of phosphate adsorption on dewatered ferric-alum residuals. J. Environ. Sci. Health Part A Toxic/Hazard. Subst. Environ. Eng. 2011, 46, 1632–1639. [CrossRef] 85. McBride, M.B. Chemisorption and precipitation reactions. In Handbook of Soil Science; Sumner, M.E., Ed.; CRC Press: Boca Raton, FL, USA, 2000; pp. 265–302. 86. Ho, Y.S.; McKay, G. Pseudo-second order model for sorption processes. Process. Biochem. 1999, 34, 451–465. [CrossRef] 87. Makris, K.C.; Sarkar, D.; Datta, R. Evaluating a drinking-water waste by-product as a novel sorbent for arsenic. Chemosphere 2006, 64, 730–741. [CrossRef] 88. Stumm, W. Chemistry of the Solid-Water Interface; John Wiley & Sons, Inc.: Chichester, UK, 1992. 89. Ong, D.C.; Kan, C.C.; Pingul-Ong, S.M.B.; de Luna, M.D.G. Utilization of groundwater treatment plant (GWTP) sludge for nickel removal from aqueous solutions: Isotherm and kinetic studies. J. Environ. Chem. Eng. 2017, 5, 5746–5753. [CrossRef] 90. de Luna, M.D.G.; Flores, E.D.; Genuino, D.A.D.; Futalan, C.M.; Wan, M.W. Adsorption of Eriochrome Black T (EBT) dye using activated carbon prepared from waste rice hulls-Optimization, isotherm and kinetic studies. J. Taiwan Inst. Chem. Eng. 2013, 44, 646–653. [CrossRef] 91. Oliveira, L.C.A.; Rios, R.; Fabris, J.D.; Sapag, K.; Garg, V.K.; Lago, R.M. Clay-iron oxide magnetic composites for the adsorption of contaminants in water. Appl. Clay Sci. 2003, 22, 169–177. [CrossRef] 92. Khalfa, L.; Bagane, M. Cadmium removal from aqueous solution by a Tunisian smectitic natural and activated clay: Thermodynamic study. J. Encapsul. Adsorpt. Sci. 2011, 1, 65–71. [CrossRef] 93. Ramesh, A.; Hasegawa, H.; Maki, T.; Ueda, K. Adsorption of inorganic and organic arsenic from aqueous solutions by polymeric Al/Fe modiﬁed montmorillonite. Sep. Purif. Technol. 2007, 56, 90–100. [CrossRef]
© 2019 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).